Procedia Engineering 55 ( 2013 ) 160 – 164
1877-7058 © 2013 The Authors. Published by Elsevier Ltd. Open access under CC BY-NC-ND license. Selection and peer-review under responsibility of the Indira Gandhi Centre for Atomic Research. doi: 10.1016/j.proeng.2013.03.236
International Conference on Cree
Creep and Creep-fatigue
, Rami Pohja, A
VTT Technical Rese
The austenitic stainless steel 316 is of current intere operating at high temperatures. Although 316 steel g and other conventional applications, improved data a especially regarding the primary to tertiary creep str update for predicting safe life to given strain and rup complex product forms. Modelling the stress depende need for long term extrapolation and limited (public temperature yield strength between casts and product present work, new creep models have been establish the Wilshire equations and logistic creep strain mode fatigue and applied to characterize the steels 316FR a
© 2013 The Authors. Published by Elsevier Ltd Gandhi Centre for Atomic Research
Keywords: Creep-fatigue; 316 stainless steel; creep; relaxati
Creep is an important limiting damage mech in design. Creep strength of steels is typically m provide data such as creep curves (strain vs. however cover new material variants and do not real service. In contrast, the growth rate of fati With increasing time spent in the cycle, the dam creep. The combined creep-fatigue (C-F) dam Miner) rule.
In this work 316 stainless steels (17% Cr modelling. The grades of interest are 316H, 316
E-mail address: Stefan.Holmstrom@vtt.fi
ep, Fatigue and Creep-Fatigue Interaction [CF-6
e Behaviour of 316 Stainless Steel
Asta Nurmela, Pekka Moilanen, Pertti Auerk
earch Centre of Finland, Espoo, Finland
est as structural material for the future Gen IV nuclear power grades have been studied for the service conditions of current and models for the long term high temperature properties are n rain and creep-fatigue response. The Gen IV technology will n pture in the temperature range of 500-750°C, and to facilitate F ence of creep strain and strain rate is particularly challenging du c domain) data. Large variation in mechanical propertiessuch t forms also need to be addressed for design and life prediction hed for predicting creep strain and rupture of 316L and316L(N) elling for improved accuracy. The models have been extended to and 316L in terms of the linear life fraction rule.
d. Selection and/or peer-review under responsibility of the
hanism for high temperature service, and must be accoun measured from isothermal constant load tests under tens time), time to failure and strain to failure. Standards t include behaviour at smaller or variable strains encounte gue damage is independent of time and the loading freq mage growth rate will increase with decreasing frequency mage is often described by the linear life fraction (Rob r–11% Ni–2% Mo) are assessed for creep and creep-f
L, 316L(N) and 316FR.
karir plants nuclear needed, need an FEA for ue to the as high n. In the ), using o creep-e Indira nted for sion, to do not ered in quency. due to binson-fatigue
© 2013 The Authors. Published by Elsevier Ltd. Open access under CC BY-NC-ND license. Selection and peer-review under responsibility of the Indira Gandhi Centre for Atomic Research.
0 1 ) log( ) log( ) log( x C t r t ¸¸ ⋅ ¹ ¨¨ © + − + = ε
Where tr is the time to rupture and x0, p and multi-linear function of temperature and stress. data set is shown in Fig.1b.
Fig. 1. (a) Creep rupture strength at 600 °C for 316FR, 316H steel against measured strains of a large multi-heat d
Material Creep Cree
316L(N) ECCC data [10,11] ECC
316FR Takahashi  -
316H NIMS  NIM
316L EN-10216-5  -
3. Predicting creep-fatigue life from creep pro
Creep-fatigue tests were conducted on 31 correspond well with the results of  as show fatigue test is shown in Fig.3. The relaxation rati
C are fitting factors. The factor x0 and p can be describe . The measured versus predicted strains of the ECCC 31
H and 316L using Wilshire model. (b) LCSP predicted creep strain for 3 data set. Note that the initial (instant) strain at loading has been removed
Data used in the assessments
ep strain Creep-Fatigue Note
CC data [10,11] - Shape parameters for strain models
Takahashi  Creep-fatigue interaction model
MS  - Creep and creep strain
models In-house data Preliminary CF
operties and cyclic peak stresses
16L stainless steel at 600°C. The creep fatigue test wn in Fig. 2. The strengthening and softening phases a io (σrelaxed/σpeak) is rapidly stabilizing to a value of about 0
(1) ed by a 16L(N) 316L(N) . results a creep 0.92.
Fig. 2. Creep fatigue and high tem
Fig. 3. Stress-strain plot of the (a) hardening phase and (b) both tens
For the 316FR steel  it can be shown tha (stress rupture curves determined from data in [7 of hold times (at a specific strain range in tensio is shown as a function of the sum of hold times constant strain range. Plotting SCF against the Miller) calculated with the test hold time (not function of peak stress (or strain range), hold tim
Fig. 4. 316FR creep fatigue data (tension hold) presented in functio
mperature low cycle fatigue results for 316L at 600°C.
) softening phase of the test at 600°C / 0.5% total strain range, 10 min h sion and compression (R=-1).
at the stress to rupture for the creep fatigue cyclic peak 7]) is closely related to the stress σref to cause rupture at th
on hold). In Fig 4, the required correction factor SCF= σp
s (¦th) showing the nearly log-linear trend of increasing S cyclic peak stress and a time-temperature parameter (L the sum), a function can be extracted to predict the SC me and temperature.
n a form where the SCF is plotted against (a) sum of hold times (th) and on of peak stress and PLM.
hold in k stress he sum peak/σref SCF at Larson-CF as a d b) as a
where k and u are constants obtained by fitting to the test data, Qc* is the apparent activation energy and σUTS is
the tensile strength at the specified temperature. The predicted cycles to end criterion is:
h h CF h f
Using the above methodology the predicted versus measured ¦th at 600°C is presented for 316FR in Fig. 5a.
The corresponding predictions for 316L (also at 600°C) using the SCF function optimized for 316FR is also shown. Predictions for 316FR can be made within a factor of 2 in comparison to measured time or number of cycles. For 316L it can be shown that directly using the SCF model (316FR behaviour) can lead to overly conservative prediction by up to a factor of 4. This indicates that the SCF function for 316FR steel cannot be directly transferred to represent the behaviour of 316L. This is though expected since the 316FR has much higher creep strength and differs in relaxation behaviour.
4. Implications of the new creep-fatigue model
The approach to creep-fatigue assessment proposed in this paper is related to an approach by  relating a hold time reduction factor Nf/Nf0 with the cycles to failure. Together with this factor and the strain range
partitioning method  it was shown for P22 steel that the impact of hold time could be predicted. The proposed new methodology is introducing a SCF function to incorporate the impact of cycling on the stress required to produce creep-fatigue failure in a time defined by the sum of hold times. The methodology appears to be robust when the stress range is within the limits of the creep data. The creep-fatigue testing at high strain ranges results in peak stresses that need creep models for shorter term properties than what are usually targeted in conventional creep modeling. A classical presentation of the creep-fatigue response by a linear life fraction diagram is shown in Fig. 5b for 316FR and 316L. The proposed creep-fatigue model has the advantage that it is does not need detailed separation of creep and fatigue components. The simple functions defining Nf enable
summation of different type of cycles to any predefined damage limit, for instance as in the Miner rule ¦[Ni(Δε,th,T)/¦Nf(Δε,th,T )] =D. This feature should be further validated for larger data sets and mixed cycle creep-fatigue. This would allow for optimised SCF functions to incorporate all desired variables.
Fig. 5. a) 316FR creep fatigue data (hold in tension) pr agreement whereas 316L life can be predicted within a fac strain ranges (0.6% & 0.8%). Note that 316L data has both terms of
The authors wish to acknowledge the suppor Finland (decision 117700) and the ECCC netwo
 ECCC Recommendations. Creep data validation and a 5: Data assessment.
 S.Holmström, P.Auerkari. Robust prediction of full c
Materials Science & Engineering for Energy Systems,
 A.Fehér et al, An interactive approach to creep behavi 34.
 B.Wilshire, M.B.Bache. Cost effective prediction of Conference (2009).
 D.W.Kim et al. Evaluation of the creep–fatigue dam
Journal of Pressure Vessels and Piping, 85(2008)p. 37
 Y.Takahashi et al, Study on creep-fatigue life predic
Nuclear Engineering and Design, 238(2008).
 Y.Takahashi et al, Long term rupture behaviour of satainless steel 316FRand their evaluation, Nuclear En  C.R.Brinkman et al., Experience in the usage of st lifetimes of uniaxial specimens of 2¼Cr-1Mo steel, ty 243, AGARD-CP-243, (1978).
 S.S.Manson et al, Creep-Fatigue analysis by strain-ran  S.R.Holdsworth et al, Factors influencing creep mode
85(2008)1-2, pp. 80-88.
 ECCC data sheet; Steel X2CrNiMoN 17-12-2 (1.4909  Data sheet on the Elevated Temperature Properties of
TB), NRIM creep data Sheet No. 6B (2000).  EN-10216-5 Seamless steel tubes for pressure purpose
resented as observed vs. predicted life. The 316 FR results show very go ctor of two for low strain range (0.5%) but may be conservative for the h h tension and compression hold; b) the creep-fatigue performance presen f the linear life fraction rule.
rt from the MATTER and NETNUC projects, the Acade ork.
assessment procedures. In: S.R.Holdsworth et al. (Eds.) ECCC Publicat
creep curves from minimal data and time to rupture model. Energy M , Vol. 1(2006)4, p. 249-255
iormodeling. Materials Science and Engineering A, Vol. 510-511 (2009
f creep design data for power plant steels. Proceedings of the ECCC
mage mechanism of Type 316L and Type 316LN stainless steelInter 78-384.
ction methods for low-carbon nitrogen-controlled 316 satinless steel (
smoothed and notched bar specimens of low-carbon nitrogen-contro
ngineering and Design, 238(2008).
train range partitioning for predicting the dependent strain-controlle ype 316 stainless steel, and Hastelloy X. AGARD Conference Proceedi
nge partitioning, NASA Technical Memorandum, NASA TMX-67838, ( el equation selection, International Journal of Pressure Vessels and Pipi
9, Type 316L(N)), 1999
f 18Cr-12Ni-Mo stainless steel tubes for boiler and heat exchangers (SU
es Part 5: Stainless Steel Tubes (2004).
ood higher nted in emy of tion Vol. Materials, 9), p. 29-C 29-Creep rnational (316FR). lled 316 ed cyclic ings No. (1971) ing, Vol. US 316H